# Scanning tunneling microscopy studies of topological ... Scanning tunneli · PDF file...

date post

08-Jul-2020Category

## Documents

view

8download

0

Embed Size (px)

### Transcript of Scanning tunneling microscopy studies of topological ... Scanning tunneli · PDF file...

Physica E 44 (2012) 912–916

Contents lists available at SciVerse ScienceDirect

Physica E

1386-94

doi:10.1

n Corr

Physics

E-m

journal homepage: www.elsevier.com/locate/physe

Scanning tunneling microscopy studies of topological insulators

Peng Cheng a, Tong Zhang a,b, Ke He b, Xi Chen a, Xucun Ma b, Qikun Xue a,b,n

a State Key Laboratory of Low-Dimensional Quantum Physics and Department of Physics, Tsinghua University, Beijing 100084, China b State Key Laboratory for Surface Physics, Institute of Physics, Chinese Academy of Sciences, Beijing 100190, China

a r t i c l e i n f o

Article history:

Received 20 September 2011

Accepted 5 November 2011 Available online 11 November 2011

77/$ - see front matter & 2011 Elsevier B.V. A

016/j.physe.2011.11.004

esponding author at: State Key Laboratory o

and Department of Physics, Tsinghua Univer

ail address: qkxue@mail.tsinghua.edu.cn (Q. X

a b s t r a c t

We summarize our recent scanning tunneling microscopy (STM) study of topological insulator thin

films grown by molecular beam epitaxy (MBE), which includes the observation of electron standing

waves on topological insulator surface and the Landau quantization of topological surface states. The

work has provided valuable information to the understanding of intriguing properties of topological

insulators, as predicted by theory.

& 2011 Elsevier B.V. All rights reserved.

1. Introduction

Topological insulator is a new class of quantum material, which possesses an energy gap in the bulk and nontrivial gapless states on the surface. The surface states are comprised of an odd number of massless Dirac cones in which crossing of two dispersion branches with opposite spins is fully protected by the time-reversal-symme- try at the Dirac point (Fig. 1). Topological insulators may provide new route to generating novel phases and quasi-particles, and may find applications in spintronics and quantum computing [1–7].

In 2009, a class of binary compounds [8–11], Bi2Se3, Bi2Te3 and Sb2Te3, was shown to be the third generation of topological insulators. Compared to Bi1�xSbx (0.07oxo0.22) alloy, the sur- face states of the Bi2Se3 family contain only a single Dirac cone, making it easier to be studied. Also, these materials are stoichio- metric compounds and hence in principle can be prepared at higher purity and quality. Finally and perhaps most importantly for applications, Bi2Se3 has a larger band gap of approximately 0.36 eV. It implies that topological behavior can sustain at room temperature. The unique properties of Bi2Se3 family have been experimentally identified by, for example angle resolved photo- emission spectroscopy (ARPES), scanning tunneling microscopy (STM) and transport measurements.

STM is a surface sensitive technique based on the concept of quantum tunneling. The atomically resolved structure of a surface can be obtained by monitoring the tunneling current in an STM. Besides its unprecedented capability to study surface topography, information on electronic structure at a given location of a sample can also be obtained. This type of measurement is called scanning tunneling spectroscopy (STS) and typically results in a plot of the

ll rights reserved.

f Low-Dimensional Quantum

sity, Beijing 100084, China.

ue).

local density of states (LDOS) as a function of energy of the sample. It has been widely used in the characterization of metals, semiconductors and superconductors. Applying it to the study of topological surface states, many intriguing properties have recently been unveiled. In this paper, we give an overview on the recent progress of STM study of topological insulators.

2. Electronic standing waves on topological insulators

In a crystal, the electronic eigen-states are described by Bloch wavefunctions ckðrÞwith energy e and wavevector k. The dispersion relation eðkÞ is usually measured by ARPES. In contrast, STM, which is a real space imaging technique, cannot be used to directly measure eðkÞ in momentum space. When disorders are introduced into a sample, the change in potential leads to the elastic electron scattering of the incident wave with a wave vector ki into kf¼kiþq, with ki and kf being on the same constant-energy contour (CEC). The quantum interference between the initial and final states results in a standing wave pattern whose spatial period is given by l¼ 2p=9q9, which are often referred to as the ‘‘Friedel oscillations’’. The phenomena can be observed by STM as modulations of the differential tunneling conductance. When the STM images of stand- ing waves are Fourier transformed, the scattering wave vector q becomes visible in the reciprocal space. This way, it simultaneously provides real-space and momentum-space information.

In 1991, Don Eigler’s group and Avouris’ group independently reported the observation of standing waves on a metal surface by STM [12,13]. Afterwards, standing waves were imaged successively on other metal (Ag, Au and Be) and semiconductor surfaces, and even on high-Tc superconductors and graphene. STM has become a powerful technique to study wavefunctions, electron scattering processes and dispersion relation of a material.

The surface states of topological insulators possess spin-polarized Dirac-cone structure and are protected by time-reversal symmetry.

www.elsevier.com/locate/physe www.elsevier.com/locate/physe dx.doi.org/10.1016/j.physe.2011.11.004 mailto:qkxue@mail.tsinghua.edu.cn dx.doi.org/10.1016/j.physe.2011.11.004

P. Cheng et al. / Physica E 44 (2012) 912–916 913

These unique characters are supposed to reflect in the scattering processes and can be explored by standing waves using STM.

In this work, stoichiometric Bi2Te3 thin films were prepared on single crystal substrate Si(1 1 1) by MBE [14]. The atomically flat morphology imaged by STM reveals high quality of our samples. The surface states of Bi2Te3 were investigated by STS, which gives a measure of the local density of states of electrons at energy eV. The differential conductance in the bulk insulating gap linearly depends on the bias and is attributed to the gapless surface states. According to the calculations, the topological states of Bi2Te3 form a single Dirac cone at the center (G point) of the surface Brillouin zone (SBZ) and the surface states around the G point overlap in energy with the bulk valence band. For this reason, the Dirac point is invisible in STS.

We deposited a small amount of Ag atoms on the clean surface of the Bi2Te3 thin film. The atomically resolved STM image reveals that a Ag atom substitutes a Bi atom in the second layer [15] The dI/dV mapping was then carried out in a region containing Ag

Fig. 1. Single Dirac cone band structure of topological insulators.

Fig. 2. (a–f) Standing waves induced by Ag trimmers on Bi2Te3(1 1 1) surface at variou current was set at 0.1 nA.

atoms. At each data point, the feedback was turned off and the bias modulation was turned onto record dI/dV. This procedure results in a series of spatial mapping of LDOS at various bias voltages.

Fig. 2(a–f) summarizes the dI/dV maps for bias voltages ranging from 50 to 400 mV. The first striking aspect of these images is the existence of standing waves in the vicinity of the Ag atoms. This phenomenon strongly supports the surface nature of topological states. For bulk states, there will be continuous ranges of wave vectors on the projected SBZ for a given energy. Usually, no distinct interference fringe can be produced by bulk states and visualized by STM.

To quantify the standing waves and obtain the scattering wave vectors, we performed fast Fourier transformation (FFT) of the dI/dV maps into the q space (Fig. 3). One important feature in the power spectra can be immediately discerned by comparing the sixfold symmetric pattern in the q space with the SBZ: the regions with high intensity are always oriented toward the G�M direc- tions, while the intensity in the G�K directions vanishes.

Such phenomena should be understood by exploring the standing wave formation mechanisms. In momentum space, ki and kf are on the same constant-energy contour (CEC) (Fig. 4). There are various directions of scattering between initial and final states. But most of these processes interfere destructively and cannot generate the observed standing waves. The interference patterns are dominated by the extremal points on the CEC, which resembles with Fermat’s principle in optics. Applying the theory to Bi2Te3 with strong warping effects, two extremal points q1 and q2 are derived: q1 along G�K and q2 alongG�M.

However, only q2 generate the observed standing waves while q1 are invisible in the power spectra. There is a simple argument to account for the disappearance of q1: the time-reversal invar- iance. q1 represents the backscattering between k and �k. These two topological states are related by the time-reversal transfor- mation: 9� k

! kS¼ bT 9 k!mS, where bT is the time-reversal operator.

It is straightforward to show that

/� k !

k9bU9 k!mS¼�/ k!m9bU9� k!kSn ¼�/� k!k9U9 k!mS¼ 0 for fermions, where U represents the impurity potential of non- magnetic Ag impurity and is a time-reversal invariant operator. Therefore, the backscattering between k and �k is quantum

s sample bias voltage. Each map is 28 nm�28 nm and has 128�128 pixels. The

Fig. 3. (a–f) FFT power spectra of the dI/dV maps in Fig. 2(a–f). SBZ in (a) is superimposed on the power spectra to indicate the directions i

*View more*